#------------------------------------------------------------------------------
#$Date: 2016-03-24 01:51:47 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179543 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/12/4501214.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4501214
loop_
_publ_author_name
'Gao, Qiang'
'Wang, Xiqu'
'Conato, Marlon T.'
'Makarenko, Tatyana'
'Jacobson, Allan J.'
_publ_section_title
;
 Microporous, Homochiral Structures Containing Iron Oxo-Clusters Supported
 by Antimony(III) Tartrate Scaffolds
;
_journal_issue                   10
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              4632
_journal_paper_doi               10.1021/cg200899w
_journal_volume                  11
_journal_year                    2011
_chemical_formula_sum            'C24 H53 Fe4 Na7 O58 Sb6'
_chemical_formula_weight         2384.49
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 120.0110(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   16.8704(7)
_cell_length_b                   21.2935(9)
_cell_length_c                   9.5632(4)
_cell_measurement_reflns_used    8101
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.31
_cell_measurement_theta_min      2.34
_cell_volume                     2974.8(2)
_computing_cell_refinement       Bruker-ApexII
_computing_data_collection       Bruker-ApexII
_computing_data_reduction        Bruker-ApexII
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    Bruker-ApexII
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.928
_diffrn_measurement_device_type  Bruker-ApexII
_diffrn_measurement_method       'narrow frame'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0322
_diffrn_reflns_av_sigmaI/netI    0.0278
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            9078
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         28.42
_diffrn_reflns_theta_min         2.34
_exptl_absorpt_coefficient_mu    3.811
_exptl_absorpt_correction_T_max  0.368
_exptl_absorpt_correction_T_min  0.332
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Blessing, 1995'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.662
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       polyhedron
_exptl_crystal_F_000             2296
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.25
_refine_diff_density_max         1.280
_refine_diff_density_min         -1.281
_refine_diff_density_rms         0.153
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.004(18)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_hydrogen_treatment    constrain
_refine_ls_matrix_type           full
_refine_ls_number_parameters     453
_refine_ls_number_reflns         6512
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.019
_refine_ls_R_factor_all          0.0303
_refine_ls_R_factor_gt           0.0301
_refine_ls_shift/su_max          0.017
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0648P)²+6.0394P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0836
_refine_ls_wR_factor_ref         0.0838
_reflns_number_gt                6442
_reflns_number_total             6512
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg200899w_si_002.cif
_cod_data_source_block           1
_cod_original_sg_symbol_H-M      C2
_cod_database_code               4501214
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sb2 Sb -0.08742(2) 0.392513(16) 0.22313(4) 0.01734(9) Uani 1 1 d .
Sb3 Sb 0.11413(2) 0.485489(15) 0.43624(4) 0.01822(8) Uani 1 1 d .
Sb4 Sb -0.10205(2) 0.560250(16) 0.20332(4) 0.01901(9) Uani 1 1 d .
Fe1 Fe 0.0000 0.47824(6) 0.0000 0.01671(18) Uani 1 2 d S
Fe2 Fe 0.0000 0.62616(5) 0.0000 0.0206(2) Uani 1 2 d S
Fe3 Fe 0.18454(5) 0.40625(3) 0.19632(9) 0.01841(16) Uani 1 1 d .
Na1 Na 0.0000 0.31049(19) 0.0000 0.0327(8) Uani 1 2 d S
Na2 Na 0.1546(3) 0.76199(17) -0.1194(5) 0.0564(9) Uani 1 1 d .
Na3 Na 0.3485(2) 0.69081(16) 0.1469(5) 0.0511(8) Uani 1 1 d .
Na4 Na 0.2081(3) 0.56385(14) 0.2241(4) 0.0431(7) Uani 1 1 d .
O1 O -0.0609(2) 0.55247(17) 0.0450(4) 0.0178(7) Uani 1 1 d .
O2 O -0.0761(3) 0.41102(17) 0.0317(4) 0.0171(7) Uani 1 1 d .
O3 O 0.1094(2) 0.47342(18) 0.2285(4) 0.0179(6) Uani 1 1 d .
O4 O -0.0277(2) 0.47942(19) 0.3160(4) 0.0179(6) Uani 1 1 d .
O5 O 0.2584(3) 0.35979(19) 0.1105(5) 0.0293(9) Uani 1 1 d .
O6 O 0.3759(4) 0.3680(3) 0.0659(8) 0.0460(13) Uani 1 1 d .
O7 O 0.2727(3) 0.4726(2) 0.2157(5) 0.0285(8) Uani 1 1 d .
O8 O 0.2412(3) 0.6016(2) 0.0131(6) 0.0330(9) Uani 1 1 d .
O9 O 0.3885(4) 0.5889(3) 0.0930(9) 0.0562(16) Uani 1 1 d .
O10 O 0.1960(3) 0.48954(19) -0.1189(5) 0.0249(8) Uani 1 1 d .
O11 O -0.0436(3) 0.6841(2) 0.1194(5) 0.0302(9) Uani 1 1 d .
O12 O 0.0034(5) 0.7421(3) 0.3381(7) 0.0572(17) Uani 1 1 d .
O13 O 0.1179(3) 0.6441(2) 0.2000(5) 0.0256(8) Uani 1 1 d .
O14 O 0.2432(3) 0.5528(2) 0.5084(6) 0.0387(10) Uani 1 1 d .
O15 O 0.2912(4) 0.6404(3) 0.6483(7) 0.0513(15) Uani 1 1 d .
O16 O 0.0701(3) 0.57678(18) 0.4001(5) 0.0240(8) Uani 1 1 d .
O17 O -0.0626(3) 0.28587(19) 0.1859(5) 0.0267(8) Uani 1 1 d .
O18 O 0.0254(3) 0.2069(2) 0.3360(6) 0.0374(11) Uani 1 1 d .
O19 O 0.0472(2) 0.37292(18) 0.3796(5) 0.0219(8) Uani 1 1 d .
O20 O 0.2629(3) 0.3949(2) 0.4442(5) 0.0282(8) Uani 1 1 d .
O21 O 0.2826(3) 0.3353(3) 0.6505(5) 0.0403(12) Uani 1 1 d .
O22 O 0.1396(3) 0.32451(18) 0.2245(4) 0.0209(7) Uani 1 1 d .
O23W O 0.3650(5) 0.6318(4) 0.3825(7) 0.0677(19) Uani 1 1 d .
O24W O 0.2269(4) 0.7391(2) 0.1580(9) 0.0535(15) Uani 1 1 d .
O25W O 0.2788(4) 0.7239(2) -0.1406(7) 0.0446(12) Uani 1 1 d .
O26W O 0.0000 0.1881(5) 0.0000 0.091(4) Uani 1 2 d S
O27W O 0.4455(5) 0.3959(6) 0.8481(10) 0.111(4) Uani 1 1 d .
O28W O 0.4409(4) 0.5685(10) 0.7960(11) 0.198(9) Uani 1 1 d .
O29W O 0.4290(9) 0.4982(10) 0.5302(13) 0.198(9) Uani 1 1 d .
O30W O 0.4503(7) 0.3686(6) 0.618(3) 0.121(9) Uani 0.50 1 d P
C1 C 0.3094(4) 0.5685(3) 0.0354(7) 0.0306(13) Uani 1 1 d .
C2 C 0.2904(4) 0.4998(3) -0.0140(7) 0.0257(11) Uani 1 1 d .
H2 H 0.3243 0.4875 -0.0681 0.031 Uiso 1 1 calc R
C3 C 0.3243(4) 0.4613(3) 0.1407(7) 0.0256(11) Uani 1 1 d .
H3 H 0.3880 0.4731 0.2159 0.031 Uiso 1 1 calc R
C4 C 0.3215(4) 0.3915(3) 0.1027(7) 0.0281(11) Uani 1 1 d .
C5 C 0.0201(5) 0.7036(3) 0.2602(7) 0.0309(13) Uani 1 1 d .
C6 C 0.1124(4) 0.6744(3) 0.3240(7) 0.0252(11) Uani 1 1 d .
H6 H 0.1588 0.7077 0.3677 0.030 Uiso 1 1 calc R
C7 C 0.1299(4) 0.6288(3) 0.4618(6) 0.0228(10) Uani 1 1 d .
H7 H 0.1190 0.6508 0.5407 0.027 Uiso 1 1 calc R
C8 C 0.2302(4) 0.6061(3) 0.5459(7) 0.0279(12) Uani 1 1 d .
C9 C 0.0108(4) 0.2629(3) 0.3044(7) 0.0237(10) Uani 1 1 d .
C10 C 0.0827(4) 0.3112(2) 0.4113(7) 0.0208(10) Uani 1 1 d .
H10 H 0.1040 0.3011 0.5247 0.025 Uiso 1 1 calc R
C11 C 0.1643(3) 0.3070(2) 0.3822(6) 0.0189(9) Uani 1 1 d .
H11 H 0.1853 0.2633 0.3985 0.023 Uiso 1 1 calc R
C12 C 0.2437(4) 0.3483(3) 0.5045(6) 0.0224(10) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Sb2 O19 97.60(15) . .
O2 Sb2 O4 88.12(14) . .
O19 Sb2 O4 75.25(14) . .
O2 Sb2 O17 86.88(15) . .
O19 Sb2 O17 72.47(15) . .
O4 Sb2 O17 146.33(14) . .
O2 Sb2 Na1 44.56(12) . .
O19 Sb2 Na1 72.53(11) . .
O4 Sb2 Na1 115.48(10) . .
O17 Sb2 Na1 44.69(12) . .
O3 Sb3 O16 97.22(16) . .
O3 Sb3 O4 88.81(13) . .
O16 Sb3 O4 75.26(16) . .
O3 Sb3 O14 86.61(16) . .
O16 Sb3 O14 71.44(16) . .
O4 Sb3 O14 145.49(16) . .
O3 Sb3 Na4 44.62(12) . .
O16 Sb3 Na4 71.67(13) . .
O4 Sb3 Na4 115.61(11) . .
O14 Sb3 Na4 44.33(14) . .
O1 Sb4 O10 97.89(15) . 2
O1 Sb4 O4 88.59(14) . .
O10 Sb4 O4 75.07(14) 2 .
O1 Sb4 O8 86.35(15) . 2
O10 Sb4 O8 72.34(15) 2 2
O4 Sb4 O8 145.95(15) . 2
O1 Sb4 Na4 44.15(12) . 2
O10 Sb4 Na4 73.48(12) 2 2
O4 Sb4 Na4 116.06(10) . 2
O8 Sb4 Na4 44.26(13) 2 2
O3 Fe1 O3 174.2(2) 2 .
O3 Fe1 O2 96.01(15) 2 2
O3 Fe1 O2 79.91(14) . 2
O3 Fe1 O2 79.91(14) 2 .
O3 Fe1 O2 96.01(15) . .
O2 Fe1 O2 91.1(2) 2 .
O3 Fe1 O1 95.41(15) 2 2
O3 Fe1 O1 89.06(14) . 2
O2 Fe1 O1 95.23(13) 2 2
O2 Fe1 O1 172.51(16) . 2
O3 Fe1 O1 89.06(14) 2 .
O3 Fe1 O1 95.41(15) . .
O2 Fe1 O1 172.51(16) 2 .
O2 Fe1 O1 95.23(13) . .
O1 Fe1 O1 78.8(2) 2 .
O3 Fe1 Na4 139.57(11) 2 .
O3 Fe1 Na4 44.79(11) . .
O2 Fe1 Na4 86.83(11) 2 .
O2 Fe1 Na4 140.48(11) . .
O1 Fe1 Na4 44.27(11) 2 .
O1 Fe1 Na4 85.73(11) . .
O3 Fe1 Na4 44.79(11) 2 2
O3 Fe1 Na4 139.57(11) . 2
O2 Fe1 Na4 140.48(11) 2 2
O2 Fe1 Na4 86.83(11) . 2
O1 Fe1 Na4 85.73(11) 2 2
O1 Fe1 Na4 44.27(11) . 2
Na4 Fe1 Na4 118.50(9) . 2
O3 Fe1 Na1 87.12(11) 2 .
O3 Fe1 Na1 87.12(11) . .
O2 Fe1 Na1 45.55(11) 2 .
O2 Fe1 Na1 45.55(11) . .
O1 Fe1 Na1 140.62(10) 2 .
O1 Fe1 Na1 140.62(10) . .
Na4 Fe1 Na1 120.75(4) . .
Na4 Fe1 Na1 120.75(4) 2 .
O13 Fe2 O13 157.8(3) . 2
O13 Fe2 O1 108.23(15) . .
O13 Fe2 O1 89.07(16) 2 .
O13 Fe2 O1 89.07(16) . 2
O13 Fe2 O1 108.23(15) 2 2
O1 Fe2 O1 79.2(2) . 2
O13 Fe2 O11 79.24(17) . .
O13 Fe2 O11 87.44(17) 2 .
O1 Fe2 O11 89.23(16) . .
O1 Fe2 O11 160.15(16) 2 .
O13 Fe2 O11 87.44(17) . 2
O13 Fe2 O11 79.24(17) 2 2
O1 Fe2 O11 160.15(16) . 2
O1 Fe2 O11 89.23(16) 2 2
O11 Fe2 O11 106.0(3) . 2
O13 Fe2 Na4 156.68(13) . 2
O13 Fe2 Na4 40.06(14) 2 2
O1 Fe2 Na4 49.43(11) . 2
O1 Fe2 Na4 92.17(12) 2 2
O11 Fe2 Na4 92.40(13) . 2
O11 Fe2 Na4 115.86(13) 2 2
O13 Fe2 Na4 40.06(14) . .
O13 Fe2 Na4 156.68(13) 2 .
O1 Fe2 Na4 92.17(12) . .
O1 Fe2 Na4 49.43(11) 2 .
O11 Fe2 Na4 115.86(13) . .
O11 Fe2 Na4 92.40(13) 2 .
Na4 Fe2 Na4 133.17(12) 2 .
O22 Fe3 O7 159.15(18) . .
O22 Fe3 O2 89.40(15) . 2
O7 Fe3 O2 107.10(16) . 2
O22 Fe3 O3 106.80(15) . .
O7 Fe3 O3 88.84(17) . .
O2 Fe3 O3 80.35(14) 2 .
O22 Fe3 O5 88.92(16) . .
O7 Fe3 O5 78.75(17) . .
O2 Fe3 O5 89.76(16) 2 .
O3 Fe3 O5 161.19(16) . .
O22 Fe3 O20 79.01(16) . .
O7 Fe3 O20 87.52(16) . .
O2 Fe3 O20 162.09(16) 2 .
O3 Fe3 O20 89.89(16) . .
O5 Fe3 O20 103.50(18) . .
O22 Fe3 Na4 154.98(13) . .
O7 Fe3 Na4 40.02(14) . .
O2 Fe3 Na4 92.41(12) 2 .
O3 Fe3 Na4 49.18(11) . .
O5 Fe3 Na4 116.03(13) . .
O20 Fe3 Na4 92.48(13) . .
O22 Fe3 Na1 40.18(12) . .
O7 Fe3 Na1 155.91(12) . .
O2 Fe3 Na1 49.58(11) 2 .
O3 Fe3 Na1 92.16(11) . .
O5 Fe3 Na1 93.53(12) . .
O20 Fe3 Na1 116.54(12) . .
Na4 Fe3 Na1 132.85(9) . .
O22 Na1 O22 164.9(3) . 2
O22 Na1 O17 95.23(13) . 2
O22 Na1 O17 87.89(13) 2 2
O22 Na1 O17 87.89(13) . .
O22 Na1 O17 95.23(13) 2 .
O17 Na1 O17 156.1(3) 2 .
O22 Na1 O2 70.29(14) . 2
O22 Na1 O2 96.92(17) 2 2
O17 Na1 O2 71.60(13) 2 2
O17 Na1 O2 131.10(17) . 2
O22 Na1 O2 96.92(17) . .
O22 Na1 O2 70.29(14) 2 .
O17 Na1 O2 131.10(17) 2 .
O17 Na1 O2 71.60(13) . .
O2 Na1 O2 68.55(18) 2 .
O22 Na1 O26W 97.54(14) . .
O22 Na1 O26W 97.54(14) 2 .
O17 Na1 O26W 78.07(13) 2 .
O17 Na1 O26W 78.07(13) . .
O2 Na1 O26W 145.73(9) 2 .
O2 Na1 O26W 145.73(9) . .
O22 Na1 C9 119.40(15) . 2
O22 Na1 C9 66.27(14) 2 2
O17 Na1 C9 25.08(15) 2 2
O17 Na1 C9 140.01(19) . 2
O2 Na1 C9 87.61(14) 2 2
O2 Na1 C9 126.83(15) . 2
O26W Na1 C9 70.28(13) . 2
O22 Na1 C9 66.27(14) . .
O22 Na1 C9 119.40(15) 2 .
O17 Na1 C9 140.01(19) 2 .
O17 Na1 C9 25.08(15) . .
O2 Na1 C9 126.83(15) 2 .
O2 Na1 C9 87.61(14) . .
O26W Na1 C9 70.28(13) . .
C9 Na1 C9 140.6(3) 2 .
O22 Na1 Fe3 33.91(11) . .
O22 Na1 Fe3 132.25(18) 2 .
O17 Na1 Fe3 85.62(10) 2 .
O17 Na1 Fe3 108.95(10) . .
O2 Na1 Fe3 36.64(9) 2 .
O2 Na1 Fe3 79.04(12) . .
O26W Na1 Fe3 126.91(6) . .
C9 Na1 Fe3 109.44(11) 2 .
C9 Na1 Fe3 94.16(11) . .
O22 Na1 Fe3 132.25(18) . 2
O22 Na1 Fe3 33.91(11) 2 2
O17 Na1 Fe3 108.95(10) 2 2
O17 Na1 Fe3 85.62(10) . 2
O2 Na1 Fe3 79.04(12) 2 2
O2 Na1 Fe3 36.64(9) . 2
O26W Na1 Fe3 126.91(6) . 2
C9 Na1 Fe3 94.16(11) 2 2
C9 Na1 Fe3 109.44(11) . 2
Fe3 Na1 Fe3 106.18(11) . 2
O22 Na1 Fe1 82.46(14) . .
O22 Na1 Fe1 82.46(14) 2 .
O17 Na1 Fe1 101.93(13) 2 .
O17 Na1 Fe1 101.93(13) . .
O2 Na1 Fe1 34.27(9) 2 .
O2 Na1 Fe1 34.27(9) . .
O26W Na1 Fe1 180.0 . .
C9 Na1 Fe1 109.72(13) 2 .
C9 Na1 Fe1 109.72(13) . .
Fe3 Na1 Fe1 53.09(6) . .
Fe3 Na1 Fe1 53.09(6) 2 .
O25W Na2 O24W 92.6(3) . .
O25W Na2 O6 129.3(2) . 4
O24W Na2 O6 90.0(2) . 4
O25W Na2 O12 120.0(3) . 2
O24W Na2 O12 130.7(2) . 2
O6 Na2 O12 94.9(3) 4 2
O25W Na2 O11 118.1(2) . 2
O24W Na2 O11 80.1(2) . 2
O6 Na2 O11 112.2(2) 4 2
O12 Na2 O11 52.73(17) 2 2
O25W Na2 O5 76.10(18) . 4
O24W Na2 O5 99.7(2) . 4
O6 Na2 O5 53.59(16) 4 4
O12 Na2 O5 122.3(2) 2 4
O11 Na2 O5 165.8(2) 2 4
O25W Na2 C4 103.8(2) . 4
O24W Na2 C4 99.3(2) . 4
O6 Na2 C4 26.46(16) 4 4
O12 Na2 C4 106.4(2) 2 4
O11 Na2 C4 138.1(2) 2 4
O5 Na2 C4 27.71(15) 4 4
O25W Na2 C5 124.5(2) . 2
O24W Na2 C5 105.9(2) . 2
O6 Na2 C5 103.1(2) 4 2
O12 Na2 C5 25.59(17) 2 2
O11 Na2 C5 27.24(16) 2 2
O5 Na2 C5 145.5(2) 4 2
C4 Na2 C5 123.1(2) 4 2
O25W Na2 Na3 48.17(18) . .
O24W Na2 Na3 44.60(17) . .
O6 Na2 Na3 119.5(2) 4 .
O12 Na2 Na3 143.1(2) 2 .
O11 Na2 Na3 98.45(16) 2 .
O5 Na2 Na3 91.02(15) 4 .
C4 Na2 Na3 110.38(17) 4 .
C5 Na2 Na3 123.44(17) 2 .
O24W Na3 O9 138.7(2) . .
O24W Na3 O17 96.6(2) . 3
O9 Na3 O17 124.5(2) . 3
O24W Na3 O23W 83.3(3) . .
O9 Na3 O23W 79.7(3) . .
O17 Na3 O23W 120.2(2) 3 .
O24W Na3 O25W 89.2(3) . .
O9 Na3 O25W 92.7(2) . .
O17 Na3 O25W 81.30(19) 3 .
O23W Na3 O25W 157.8(2) . .
O24W Na3 O8 86.0(2) . .
O9 Na3 O8 53.91(17) . .
O17 Na3 O8 161.2(2) 3 .
O23W Na3 O8 78.6(2) . .
O25W Na3 O8 80.09(19) . .
O24W Na3 O18 129.1(2) . 3
O9 Na3 O18 85.47(19) . 3
O17 Na3 O18 52.07(15) 3 3
O23W Na3 O18 82.4(2) . 3
O25W Na3 O18 118.0(2) . 3
O8 Na3 O18 137.4(2) . 3
O24W Na3 C1 112.7(2) . .
O9 Na3 C1 26.58(18) . .
O17 Na3 C1 148.4(2) 3 .
O23W Na3 C1 76.7(2) . .
O25W Na3 C1 87.2(2) . .
O8 Na3 C1 27.38(17) . .
O18 Na3 C1 111.0(2) 3 .
O24W Na3 C9 111.9(2) . 3
O9 Na3 C9 107.7(2) . 3
O17 Na3 C9 26.97(16) 3 3
O23W Na3 C9 98.8(2) . 3
O25W Na3 C9 103.4(2) . 3
O8 Na3 C9 161.6(2) . 3
O18 Na3 C9 25.63(16) 3 3
C1 Na3 C9 134.2(2) . 3
O24W Na3 Na2 44.8(2) . .
O9 Na3 Na2 121.3(2) . .
O17 Na3 Na2 91.88(15) 3 .
O23W Na3 Na2 123.2(2) . .
O25W Na3 Na2 44.64(16) . .
O8 Na3 Na2 76.79(15) . .
O18 Na3 Na2 143.95(16) 3 .
C1 Na3 Na2 100.35(17) . .
C9 Na3 Na2 118.54(16) 3 .
O24W Na3 Na4 70.57(16) . .
O9 Na3 Na4 71.15(17) . .
O17 Na3 Na4 158.95(17) 3 .
O23W Na3 Na4 43.71(17) . .
O25W Na3 Na4 114.13(17) . .
O8 Na3 Na4 38.25(13) . .
O18 Na3 Na4 123.27(17) 3 .
C1 Na3 Na4 50.95(14) . .
C9 Na3 Na4 142.49(17) 3 .
Na2 Na3 Na4 90.18(11) . .
O13 Na4 O7 168.5(3) . .
O13 Na4 O8 95.02(18) . .
O7 Na4 O8 86.58(16) . .
O13 Na4 O14 87.84(18) . .
O7 Na4 O14 95.91(18) . .
O8 Na4 O14 153.1(2) . .
O13 Na4 O1 72.35(16) . 2
O7 Na4 O1 97.30(18) . 2
O8 Na4 O1 73.20(15) . 2
O14 Na4 O1 132.52(19) . 2
O13 Na4 O3 99.40(18) . .
O7 Na4 O3 71.43(15) . .
O8 Na4 O3 132.09(18) . .
O14 Na4 O3 73.26(15) . .
O1 Na4 O3 68.35(15) 2 .
O13 Na4 O23W 94.2(2) . .
O7 Na4 O23W 97.2(2) . .
O8 Na4 O23W 74.20(19) . .
O14 Na4 O23W 78.9(2) . .
O1 Na4 O23W 143.3(2) 2 .
O3 Na4 O23W 148.4(2) . .
O13 Na4 C1 118.15(19) . .
O7 Na4 C1 65.22(16) . .
O8 Na4 C1 23.97(16) . .
O14 Na4 C1 138.9(2) . .
O1 Na4 C1 87.52(16) 2 .
O3 Na4 C1 126.63(17) . .
O23W Na4 C1 68.53(18) . .
O13 Na4 C8 67.00(17) . .
O7 Na4 C8 118.34(19) . .
O8 Na4 C8 139.7(2) . .
O14 Na4 C8 23.26(17) . .
O1 Na4 C8 128.01(18) 2 .
O3 Na4 C8 87.57(15) . .
O23W Na4 C8 71.72(19) . .
C1 Na4 C8 140.2(2) . .
O13 Na4 Fe2 35.15(12) . .
O7 Na4 Fe2 133.89(18) . .
O8 Na4 Fe2 86.65(14) . .
O14 Na4 Fe2 109.76(14) . .
O1 Na4 Fe2 37.51(9) 2 .
O3 Na4 Fe2 79.99(13) . .
O23W Na4 Fe2 124.4(2) . .
C1 Na4 Fe2 109.17(14) . .
C8 Na4 Fe2 95.14(14) . .
O13 Na4 Fe3 135.18(18) . .
O7 Na4 Fe3 34.72(11) . .
O8 Na4 Fe3 108.90(14) . .
O14 Na4 Fe3 86.93(14) . .
O1 Na4 Fe3 78.97(12) 2 .
O3 Na4 Fe3 36.97(9) . .
O23W Na4 Fe3 128.1(2) . .
C1 Na4 Fe3 93.69(14) . .
C8 Na4 Fe3 108.87(14) . .
Fe2 Na4 Fe3 107.47(11) . .
O13 Na4 Sb4 88.43(14) . 2
O7 Na4 Sb4 85.08(13) . 2
O8 Na4 Sb4 42.23(11) . 2
O14 Na4 Sb4 164.58(18) . 2
O1 Na4 Sb4 32.57(9) 2 2
O3 Na4 Sb4 92.62(12) . 2
O23W Na4 Sb4 116.27(16) . 2
C1 Na4 Sb4 55.06(12) . 2
C8 Na4 Sb4 155.07(16) . 2
Fe2 Na4 Sb4 60.47(6) . 2
Fe3 Na4 Sb4 85.20(7) . 2
Sb4 O1 Fe2 120.57(18) . .
Sb4 O1 Fe1 129.51(18) . .
Fe2 O1 Fe1 101.04(16) . .
Sb4 O1 Na4 103.29(16) . 2
Fe2 O1 Na4 93.06(14) . 2
Fe1 O1 Na4 101.54(16) . 2
Sb2 O2 Fe3 122.20(18) . 2
Sb2 O2 Fe1 129.58(19) . .
Fe3 O2 Fe1 99.85(15) 2 .
Sb2 O2 Na1 103.13(15) . .
Fe3 O2 Na1 93.78(14) 2 .
Fe1 O2 Na1 100.18(15) . .
Sb3 O3 Fe3 122.14(18) . .
Sb3 O3 Fe1 129.34(17) . .
Fe3 O3 Fe1 99.88(15) . .
Sb3 O3 Na4 102.75(16) . .
Fe3 O3 Na4 93.84(13) . .
Fe1 O3 Na4 101.06(16) . .
Sb3 O4 Sb2 118.00(18) . .
Sb3 O4 Sb4 117.63(18) . .
Sb2 O4 Sb4 118.41(16) . .
C4 O5 Fe3 116.9(4) . .
C4 O5 Na2 87.2(4) . 4_545
Fe3 O5 Na2 147.3(2) . 4_545
C4 O6 Na2 92.9(4) . 4_545
C3 O7 Fe3 117.3(3) . .
C3 O7 Na4 127.2(3) . .
Fe3 O7 Na4 105.27(19) . .
C1 O8 Sb4 110.8(4) . 2
C1 O8 Na4 103.7(4) . .
Sb4 O8 Na4 93.51(18) 2 .
C1 O8 Na3 88.5(3) . .
Sb4 O8 Na3 150.8(2) 2 .
Na4 O8 Na3 103.3(2) . .
C1 O9 Na3 93.2(5) . .
C2 O10 Sb4 123.0(4) . 2
C5 O11 Fe2 115.3(4) . .
C5 O11 Na2 91.1(4) . 2
Fe2 O11 Na2 151.1(2) . 2
C5 O12 Na2 94.5(5) . 2
C6 O13 Fe2 116.6(4) . .
C6 O13 Na4 127.0(4) . .
Fe2 O13 Na4 104.8(2) . .
C8 O14 Sb3 111.3(4) . .
C8 O14 Na4 104.4(4) . .
Sb3 O14 Na4 93.23(19) . .
C7 O16 Sb3 123.5(3) . .
C9 O17 Sb2 113.4(4) . .
C9 O17 Na3 93.8(3) . 3_445
Sb2 O17 Na3 132.7(2) . 3_445
C9 O17 Na1 98.2(3) . .
Sb2 O17 Na1 94.25(17) . .
Na3 O17 Na1 120.3(2) 3_445 .
C9 O18 Na3 86.4(4) . 3_445
C10 O19 Sb2 122.9(3) . .
C12 O20 Fe3 116.7(3) . .
C11 O22 Fe3 117.1(3) . .
C11 O22 Na1 126.2(3) . .
Fe3 O22 Na1 105.90(19) . .
Na3 O23W Na4 97.4(2) . .
Na3 O24W Na2 90.6(2) . .
Na2 O25W Na3 87.2(2) . .
O9 C1 O8 124.1(6) . .
O9 C1 C2 119.2(6) . .
O8 C1 C2 116.7(5) . .
O9 C1 Na3 60.2(4) . .
O8 C1 Na3 64.1(3) . .
C2 C1 Na3 176.1(4) . .
O9 C1 Na4 123.1(5) . .
O8 C1 Na4 52.4(3) . .
C2 C1 Na4 93.4(3) . .
Na3 C1 Na4 84.2(2) . .
O10 C2 C1 110.9(5) . .
O10 C2 C3 110.4(4) . .
C1 C2 C3 107.2(5) . .
O7 C3 C4 109.7(4) . .
O7 C3 C2 112.1(5) . .
C4 C3 C2 109.8(5) . .
O6 C4 O5 123.5(6) . .
O6 C4 C3 121.5(6) . .
O5 C4 C3 115.0(5) . .
O6 C4 Na2 60.6(4) . 4_545
O5 C4 Na2 65.1(3) . 4_545
C3 C4 Na2 165.2(4) . 4_545
O12 C5 O11 121.2(7) . .
O12 C5 C6 122.5(6) . .
O11 C5 C6 116.2(5) . .
O12 C5 Na2 59.9(4) . 2
O11 C5 Na2 61.7(3) . 2
C6 C5 Na2 175.9(4) . 2
O13 C6 C5 110.1(5) . .
O13 C6 C7 111.7(5) . .
C5 C6 C7 109.0(5) . .
O16 C7 C6 110.2(4) . .
O16 C7 C8 109.8(5) . .
C6 C7 C8 109.5(5) . .
O14 C8 O15 124.7(6) . .
O14 C8 C7 116.2(5) . .
O15 C8 C7 119.1(6) . .
O14 C8 Na4 52.3(3) . .
O15 C8 Na4 127.2(5) . .
C7 C8 Na4 91.0(3) . .
O18 C9 O17 125.0(5) . .
O18 C9 C10 119.7(5) . .
O17 C9 C10 115.3(5) . .
O18 C9 Na3 68.0(3) . 3_445
O17 C9 Na3 59.2(3) . 3_445
C10 C9 Na3 162.8(4) . 3_445
O18 C9 Na1 118.3(4) . .
O17 C9 Na1 56.8(3) . .
C10 C9 Na1 93.7(3) . .
Na3 C9 Na1 95.38(18) 3_445 .
O19 C10 C9 111.9(4) . .
O19 C10 C11 109.7(4) . .
C9 C10 C11 108.9(4) . .
O22 C11 C10 111.7(4) . .
O22 C11 C12 110.0(4) . .
C10 C11 C12 110.3(4) . .
O21 C12 O20 125.1(5) . .
O21 C12 C11 119.7(5) . .
O20 C12 C11 115.2(4) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sb2 O2 1.973(4) .
Sb2 O19 2.043(4) .
Sb2 O4 2.082(4) .
Sb2 O17 2.368(4) .
Sb2 Na1 3.596(2) .
Sb3 O3 1.965(3) .
Sb3 O16 2.048(4) .
Sb3 O4 2.076(3) .
Sb3 O14 2.402(5) .
Sb3 Na4 3.554(3) .
Sb4 O1 1.963(4) .
Sb4 O10 2.037(4) 2
Sb4 O4 2.084(4) .
Sb4 O8 2.390(4) 2
Sb4 Na4 3.549(3) 2
Fe1 O3 2.039(3) 2
Fe1 O3 2.039(3) .
Fe1 O2 2.044(4) 2
Fe1 O2 2.044(4) .
Fe1 O1 2.045(4) 2
Fe1 O1 2.045(4) .
Fe1 Na4 3.565(4) .
Fe1 Na4 3.565(4) 2
Fe1 Na1 3.572(4) .
Fe2 O13 1.988(4) .
Fe2 O13 1.988(4) 2
Fe2 O1 2.036(4) .
Fe2 O1 2.036(4) 2
Fe2 O11 2.051(4) .
Fe2 O11 2.051(4) 2
Fe2 Na4 3.339(3) 2
Fe2 Na4 3.339(3) .
Fe3 O22 1.970(4) .
Fe3 O7 1.992(4) .
Fe3 O2 2.031(4) 2
Fe3 O3 2.034(4) .
Fe3 O5 2.057(4) .
Fe3 O20 2.072(4) .
Fe3 Na4 3.374(3) .
Fe3 Na1 3.395(3) .
Na1 O22 2.278(4) .
Na1 O22 2.278(4) 2
Na1 O17 2.536(4) 2
Na1 O17 2.536(4) .
Na1 O2 2.591(5) 2
Na1 O2 2.591(5) .
Na1 O26W 2.607(12) .
Na1 C9 3.001(6) 2
Na1 C9 3.001(6) .
Na1 Fe3 3.395(3) 2
Na2 O25W 2.349(7) .
Na2 O24W 2.351(9) .
Na2 O6 2.426(7) 4
Na2 O12 2.466(7) 2
Na2 O11 2.502(5) 2
Na2 O5 2.524(6) 4
Na2 C4 2.780(8) 4
Na2 C5 2.842(8) 2
Na2 Na3 3.339(5) .
Na3 O24W 2.344(7) .
Na3 O9 2.404(7) .
Na3 O17 2.434(5) 3
Na3 O23W 2.471(8) .
Na3 O25W 2.491(7) .
Na3 O8 2.491(5) .
Na3 O18 2.626(6) 3
Na3 C1 2.767(7) .
Na3 C9 2.828(7) 3
Na3 Na4 3.901(5) .
Na4 O13 2.222(5) .
Na4 O7 2.249(5) .
Na4 O8 2.482(5) .
Na4 O14 2.487(6) .
Na4 O1 2.540(5) 2
Na4 O3 2.559(5) .
Na4 O23W 2.718(8) .
Na4 C1 3.045(7) .
Na4 C8 3.045(6) .
Na4 Sb4 3.549(3) 2
O1 Na4 2.540(5) 2
O2 Fe3 2.031(4) 2
O5 C4 1.294(7) .
O5 Na2 2.524(6) 4_545
O6 C4 1.241(7) .
O6 Na2 2.426(7) 4_545
O7 C3 1.398(7) .
O8 C1 1.273(8) .
O8 Sb4 2.390(4) 2
O9 C1 1.240(8) .
O10 C2 1.411(6) .
O10 Sb4 2.037(4) 2
O11 C5 1.301(8) .
O11 Na2 2.502(5) 2
O12 C5 1.231(8) .
O12 Na2 2.466(7) 2
O13 C6 1.393(7) .
O14 C8 1.241(8) .
O15 C8 1.242(7) .
O16 C7 1.413(6) .
O17 C9 1.285(7) .
O17 Na3 2.434(5) 3_445
O18 C9 1.226(8) .
O18 Na3 2.626(6) 3_445
O19 C10 1.414(6) .
O20 C12 1.268(7) .
O21 C12 1.242(7) .
O22 C11 1.399(6) .
C1 C2 1.521(8) .
C2 C3 1.530(8) .
C3 C4 1.526(8) .
C4 Na2 2.780(8) 4_545
C5 C6 1.494(9) .
C5 Na2 2.842(8) 2
C6 C7 1.542(8) .
C7 C8 1.545(8) .
C9 C10 1.527(8) .
C9 Na3 2.828(7) 3_445
C10 C11 1.537(7) .
C11 C12 1.540(7) .
